**HAL Id: jpa-00236673**

**https://hal.archives-ouvertes.fr/jpa-00236673**

### Submitted on 1 Jan 1962

**HAL** is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

### L’archive ouverte pluridisciplinaire **HAL, est** destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

**Hyperfine field in metals and alloys**

### W. Marshall, C.E. Johnson

**To cite this version:**

### W. Marshall, C.E. Johnson. Hyperfine field in metals and alloys. J. Phys. Radium, 1962, 23 (10),

### pp.733-737. �10.1051/jphysrad:019620023010073300�. �jpa-00236673�

### HYPERFINE FIELD IN METALS AND ALLOYS

### By W. MARSHALL and C. E. JOHNSON,

### A. E. R. E. Harwell, Berkshire, England.

### Resumé. 2014 _{On passe }

^{en }

^{revue }

### les différentes contributions

au### champ magnétique

^{au }

### noyau dans les métaux et les alliages ferromagnetiques ^{et } paramagnétiques. ^{La } comparaison

^{avec }

^{les}

### résultats expérimentaux ^{montre } la faiblesse de la théorie, ^{ainsi } l’approche empirique ^{du } sujet ^{est}

### pour l’instant la meilleure méthode possible. Néanmoins les

mesures### de champ hyperfines peuvent

### fournir des reformations utiles. Par exemple,

^{en }

### utilisant l’effet Mössbauer 2014 qui permet ^{d’observer}

### des distributions de champs trop larges pour être visibles

^{en }

### RMN -

on### peut

^{en }

### principe ^{obtenir}

### des informations

sur### les systèmes magnétiques désordonnées qui

^{ne }

^{sont } fournis par

^{aucune }

### autre

### technique.

### Abstract.

^{2014 }

### A review is given of the contributions to the magnetic ^{field at } nuclei in ferro-

### magnetic ^{and } paramagnetic ^{metals } ^{and } alloys. Comparison ^{with } experimental data shows the weakness of the theory ^{and } ^{hence }

^{an }

### empirical approach ^{to the } subject ^{is } ^{the } ^{best } possible ^{at } ^{the} present time. Nevertheless hyperfine field measurements _{may } give ^{useful } information. For

### example using the Mössbauer effect, where distributions of fields too broad to be

seen### by ^{NMR}

can

### be observed, information

on### random magnetic assemblies which cannot be obtained by any other technique may in principle ^{be } investigated.

### 23,

### The effective magnetic ^{field } acting

^{on a }

^{nucleus}

### in a solid can be discussed in various ways but it is best to regard ^{it }

^{as }

^{the } ^{sum } ^{of the } following

### contributions [1].

### (a) The usual internal field which, ^{for } ^{cubic} materials, ^{is}

### where Ho ^{is } thg ^{external } field, - D.H the dema-

### gnetising field and 47u M/3 the Lorentz field. The Lorentz term has the coefficient 4n j3 only ^{in } ^{cubic} symmetry but in all _{cases, } even in crystals ^{of low} symmetry, ^{Hint } ^{is known } exactly. In parama-

### gnetic ^{metals } ^{Hint } is the main field but in ferro-

### magnets ^{it is } important only because the appli-

### cation of

an### external field Ho of ^{known } sign

### enables the sign ^{of the } ^{effective } hyperfine ^{field } ^{to}

### be determined.

### (b) ^{The field } produced by the orbital magnetic

### moment on the parent ^{atom}

### where y is the Bohr magneton ^{and } ^{the } expectation

### values refer, ^{for } example ^{to } ^{the 3d } ^{electrons } ^{of }

^{a}

### transition metal

or### the 4 f electrons of

a### rare earth metal.

### (c) ^{The field } produced by ^{the } dipolar interaction with the spin ^{moment }

^{on }

^{the } parent ^{atom}

### In

a### cubic metal in the absence ouf spin ^{orbit} coupling this field is

zero ### and if the crystal ^{is } ^{non-}

### cubic then the resulting field may very well be small enough ^{to } ^{be } neglected ^{for } ^{most } purposes.

### In the rare earth metals, however, ^{because } ^{L is } ^{not} quenched the electron density ^{can } ^{have } ^{an } asym-

### metrical shape ^{with } ^{a } principal ^{axis } given by ^{the S}

### vector. In that

case### (3)

^{can }

^{be } quite large.

### (d) ^{The field } proportional ^{to } ^{the } spin density ^{at}

### the nucleus.

### This field arises through ^{the well } ^{known } ^{Fermi}

### contact interaction.

### The relative importance ^{of } these contributions varies from one type ^{of } ^{material } ^{to } ^{another } ^{and it}

### is therefore convenient to discuss the field under two headings : (1) ferromagnetic metals and alloys

### of the first transition period ; (2) paramagnetic

### metals and alloys of the first transition period.

### We shall see that the problem ^{of } interpretation

### which arise are essentially similar and that

we### may therefore regard measurements of the hyperfine

### field in ferromagnets using, say, ^{the } Môssbauer

### technique

^{as }

^{the } equivalent ^{of } Knight bhift ^{measu-}

### rements by ^{N. } ^{M. } ^{R. in the } paramagnetic ^{materials.}

### In contrast to ^{these } ^{cases } ^{there } ^{are } very few diffi- culties of interpretation connected with the rare

### earth metals and therefore

we### shall not discuss them.

### 1. Ferromagnetie ^{metals } ^{and } alloys.- In these materials experiment shows that the effective field is large, usually ^{of the } order of several hundred

### kilogauss, ^{and } usually ^{is } negative. ^{Therefore } ^{Hint}

### is of little importance except ^{to } establish the sign

### of the field. The orbital term HL ^{is } more conve-

### niently expressed

^{as}

### and, ^{because } g is close ^{to } 2 in these materials, ^{is}

### Article published online by EDP Sciences and available at http://dx.doi.org/10.1051/jphysrad:019620023010073300

### 734

### small compared ^{to } ^{the } ^{total. } Using ^{a } typical

### value of g

^{- }

### 2 r-J 0.1 we find HL is of the order of + 70 kg ^{in Fe. } Experiment ^{on } ^{Fe shows } ^{that}

### the total field is - 340 kg [2] ^{and } hence, ^{since } HD is zero for Fe, ^{a } ^{field } of the order of - 410 kg

### must come from the spin density ^{at } ^{the } Fe nucleus.

### But before discussing ^{this } ^{term } ^{in } ^{detail }

^{we }

^{first}

### comment that HD ^{is } ^{not } ^{zero } ^{in } hexagonal ^{Co.}

### In a crystal ^{with } ^{axial } symmetry, ^{such } ^{as } ^{hexa-} gonal ^{Co } (3) ^{can } ^{be } put in the form

### where 0 is the angle between the spin ^{direction } ^{and}

### the principal ^{axis. } ^{The } ^{best } ^{way } ^{to } ^{estimate } ^{this}

### term is to measure the quadrupole interaction

### where q

^{= }

### 2 r-3 > 3 cos 2 0 -1 > ^{8 } >.

### Hence HD is simply 03BCq. In this way G. Perlow [3],

### who has measured the quadrupole splitting ^{OfS7 } ^{Fe}

### dissolved in hexagonal ^{Co } using ^{the } ^{Mossbauer} effect, ^{concludes } ^{that } HD is smaller than 3 kg ^{in}

### this case. We conclude that even in an anisotropic crystal ^{like } hexagonal Co that nevertheless the electrons are distributed around the nucleus with a

### high symmetry ^{and } ^{so } ^{HD } ^{is in } practice, quite negligible.

### It follows that the hyperfine ^{field } ^{in } ^{a } ^{ferro-} magnet is almost entirely ^{due } ^{to. } ^{the } spin density

### at the nucleus. This is a well defined quantity ^{but}

### is difficult to interpret ^{because } ^{our } knowledge ^{of}

### these metals and alloys is poor and ^{our } under-

### standing ^{of how } spin density ^{is } produced ^{at } ^{the}

### nucleus is weak.

### In paramagnetic ^{salts } the mechanism by ^{which } ^{a} magnetic ^{moment } of the 3d electrons could give ^{rise}

### to a spin polarization ^{at } ^{the } ^{nucleus } ^{has } ^{been}

### underEtood in principle ^{for } some time. In physical

### terms the mechanism arises because the exchange

### interaction between the polarized 3d electrons and the inner core s électrons, ls, ^{2s and } 3s, produces ^{an} asymmetry ^{between } ^{the } ^{inner } ^{electrons } depending

### upon their spin orientation ; ^{and } ^{because } ^{of this} asymmetry ^{the } ^{inner } ^{core } ^{electrons } ^{can } give ^{a } ^{net} spin density which, though ^{zero on } average, ^{can} have a non-zero value at the nucleus. A good ^{for-}

### mulation of the problem ^{and } ^{a } description ^{of the}

### calculations which it would be _{necessary } to carry out was given by Abragam, ^{Horowitz } ^{and } Pryce [4]

### They regard ^{the } problem ^{as one } ^{of } performing ^{the} appropriate configuration interaction calculation.

### To illustrate their argument ^{let } ^{us } ^{consider } ^{the} simple ^{three } ^{electron } ^{case } of Li where the Hartree- Fock wavefunction for the first excited state would be written as

### where the brackets { } ^{stand for }

^{a }

^{properly } ^{norma-}

### lised déterminant. The spin density ^{at } thenucleus ^{is}

### zero according ^{to } (8) because the 1s orbitals have

### paired spins ^{and } 2p ^{orbital } ^{has } ^{zero } amplitu ^{deat the}

### nucleus. But to improve ^{on } ^{the } Hartree-Fock wavefunction we must add other configurations

### and Abragam, Horowitz and Pryce point ^{out } ^{that}

### the configuration ^{where } ^{one } ^{of the 1s } ^{electrons } ^{is} promoted ^{into } ^{some } higher state, Rs, ^{is } specially important ^{for } ^{a } discussion of spin density. They

### therefore took a wavefunction of the form

### where the function Rs is to be determined by ^{a}

### variational calculation and the precise ^{form of } (9)

### is dictated by ^{the } requirement that the total spin S2 be ^{a } good quantum ^{number. } ^{The } ^{wave-} function (9) ^{does } give ^{a } spin density ^{at } the nucleus which is 2 ls(O) .Rs(o).

### Unfortunately calculations of this type ^{are } ^{diffi-}

### cult to perform and therefore many calculations have been made (e.g. by ^{Freeman } ^{and } ^{Watson } [5]) using the Unrestricted Hartree-Fock method which

### simply assumes a wavefunction of the type (8)

### with the radial form of 1sa différent from that of 1sa. This method is simple ^{but } ^{does } ^{not } give eigenstates of S2 and is therefore open ^{to } criticism.

### Some discussion of the validity ^{of the } Unrestricted Hartree-Fock method has been given by

### Marshall [6] ^{but } ^{no } ^{clear } ^{decision } ^{seems } possible ^{at}

### the present ^{time. In } ^{view } ^{of this } ^{we } ^{should } regard

### the Unrestricted Hartree-Fock method as a heu- ristic method capable ^{of } indicating ^{trends } ^{and}

### orders of magnitude : ^{this } point of view has been

### emphasised by ^{Watson } ^{and } Freeman themselves.

### In principle it is clear that the same mechanism

### can give ^{rise } ^{to } ^{core } polarization in metals but because the ‘’ 3d electrons " are described by ^{diffe-}

### rent wavefunctions in the metal it is impossible ^{to}

### make _{any } estimate whether the eff ect is increased

### or decreased in metals. No calculations have yet

### been performed ^{on } anything other than isolated ions but Watson and Freeman have shown the effect is remarkably ^{sensitive } ^{to } ^{the } ^{extent } ^{of the } ^{3d}

### radial function.

### One point ^{of } importance upon ^{which } ^{we } ^{do } ^{not}

### even have qualitative information is the relative

### importance ^{of } ^{3d } ^{and 4s } magnetisations ^{in } pro-

### ducing ^{core } polarization. ^{In } ^{a } ferromagnet ^{such}

as

### Fe we can expect ^{a } ^{4s } magnetisation ^{of the}

### order of 0.1 to 0.2 II per ^{atom } (it may well be

### négative) ^{and }

^{we }

^{have } ^{no } assessment of the core

### polarization this would produce.

### Although ^{core } polarization probably provides

### the bulk of the hyperfine ^{field in } ferromagnetic

### metals a further contribution must also be made

### directly by ^{the 4s } conduction électrons. These

### électrons are polarized by ^{both } by the exchange

### intér action with the 3d électrons (a positive ^{term)}

### and by ^{the } complicated eff ects of mixing ^{with the}

### 3d band. These mixing eff ects have been descrif bed by ^{Anderson } [7] but without a firm idea o-

### the band structure of these metals it seems impos-

### sible to make a quantitative estimate of them.

### Another difficulty is that the spin density ^{even } ^{in}

a

### free electron gas ^{can } be very non-uniform. This has been studied by ^{Yosida } [8] ^{who } ^{has } pointed ^{out}

### that in some cases the spin density ^{can } ^{fluctuate}

### from one part of the unit cell to another by ^{an}

### order of magnitude ^{more } ^{than } ^{the } ^{mean } ^{value.}

### This suggestion ^{is } ^{borne } ^{out } by ^{the } experiments ^{of} Gossard, ^{Jaccarino } ^{and } ^{Wernick } [9] ^{on } ^{the Laves} phases ^{RAI } ^{where R } ^{is } ^{a rare } ^{earth } ^{atom. } They

### find that the Knight ^{shift } ^{at } ^{the } ^{aluminium } ^{nucleus}

### is negative although ^{the } exchange ^{effect } ^{between}

### the rare earth ions and the conduction electrons is

### certainly positive.

### This point ^{is } ^{of } great importance ^{is } considering

### the results on the hyperfine fields of diamagnetic

### atoms dissolved in

a### ferromagnet. Many ^{measu-}

### rements of this kind have been made and some of the data are summarised in Table I, together ^{with}

### TABLE 1

### Note that H and S >

are### of opposite signs.

^{’ }

^{. }

### The sign ^{of } ^{H } ^{is } ^{most } directly determined in Môssbauer measurements (e.g. 119Sn, [18] 197Au)

1l 7 ### [19], Samoilev et al deduce sign the from the assymmetry ^{of } p-emission from oriented nuclei. They ^{obtain } negative fields for 198Au in Fe and Ni [20]. ^{The } positive sign for 122Sb is not yet ^{definite.}

### The relative values of H for 197Au in Fe, ^{Co and Ni }

^{are }

^{known }

^{more }

### accurately than the absolute values, ^{and }

^{are}

### proportional to the saturation magnetisation (Roberts and Thomson [10]). ^{The } positive sign has been measured by Shirley ^{and al. } [19].

### The data for 27 AI and 63Cu

were### obtained by ^{Koi et } ^{al. } [21].

### estimates of the spin ^{of } ^{the } conduction electron in the impurity ^{unit } cell calculated

on ### the assump- tion that for the diamagnetic ^{atom } ^{the } ^{entire } ^{field}

### comes from a Knight shift eff ect via the conduction electrons. We notice that the mean spin ^{values} required ^{to } ^{fit the } experimental data vary widely

### from one atom to another both in magnitude ^{and} sign, ^{and in } ^{view } ^{of the } expected flictuations in the

### spin density ^{this is } ^{not } surprising. [However

### Roberts and Thomson [10] ^{find that } ^{th’e } hyperfine

### field on 197Au dissolved in iron cobalt and nickel is accurately proportional ^{to } ^{the } saturation _{magne-} tisation of the spécimen.]

### In trying ^{to } interpret hyperfine ^{fields } ^{measured}

### for magnetic ^{atoms } ^{the } unsatisfactory ^{unders-} tanding ^{of the } theory ^{reduces } ^{us } ^{to } trying ^{to } ^{fit the}

### data to empirical rules. The simplest ^{rule } ^{we}

### could postulate is that the field should be propor- tional to the magnetic ^{moment }

^{on }

^{the } ^{atom.’ } ^{For}

### some ordered alloys this rule appears ^{to } hold ; ^{for} example in the ordered alloy Fe3AI ^{there } ^{are } ^{two}

### ion sites whose hyperfine ^{fields } [11] ^{and atomic}

### moments [12]

^{are}

### The value of H /{L ^{for } pure ion is 150, ^{which}

### agrees well with the last column above. However,

### such agreement appears ^{to } be confined to isolated

### examples.

### Figure 1 shows the variation of the hyperfine

### field at 57Fe nuclei

as### a function of composition ^{in}

### iron alloys ^{with } cobalt, nickel, chromium, ^{vana-}

### dium and aluminium [11]. Also shown are the

### magnetic ^{moment } yfe ^{localised } ^{on } ^{the iron } ^{atoms} (determined ^{from } ^{diffuse } scattering ^{of } ^{neutrons } [13]

### or from the saturation magnetisation ^{for } ^{Fe-Ai}

### where the aluminium contributes no moment) ^{and}

### the average atomic moment y (determined ^{from}

### saturation magnetisation measurements). ^{The}

### three quantities HF9, 03BCFe and p. ^{have been } ^{norma-}

### lised in terms of the values for pure iron : ^{It is} clear that the simple ^{rule does } ^{not } ^{hold } ^{in } general.

### In all these cases it is observed that the hyperfine

### field varies with alloys concentration in a way which is intermediate between that of the iron moment itself and the mean moment of the sample

### as a whole. However, ^{no } ^{solution } ^{of the } ^{form}

### HFe

^{= }

_{a03BCFe } + b03BC ^{with } constant a and b can be found to fit all the alloys. Part of the discre-

### pancies may be accounted for the changes ^{in } ^{the}

### number of conduction electrons with alloy ^{compo-}

### sition. For example ^{in the } ^{Fe-Ai } system ^{the}

### 736

### FIG. 1.

^{- }

### The variation of the hyperfine ^{field }

^{as }

### iron nuclei HFe, ^{the } magnetic ^{moment }

^{on }

### iron atoms _{03BCFe} and the average magnetic moment fi ^{for iron } alloys ^{Values }

^{are }

### normalised to those of pure iron.

### Mossbauer spectrum ^{shows } ^{a } positive isomer shift with increasing ^{aluminium } ^{content } [11] ^{corres-} ponding ^{to }

^{a }

### drecrease in the number of con-

### duction electrons and hence a more rapid ^{fall } ^{in}

### the hyperfine field than that expected ^{for }

^{a}

### decrease in y ^{alone. } Another result of alloying

### which may affect the hyperfine ^{field is } ^{a } charge

### in the density ^{of } states, ^{which } may be inferred

### from ’the linear contribution ^{to } ^{the low } tempe-

### rature specific ^{heat. } Perhaps ^{when }

^{more com-}

### plete ^{data } ^{for } alloys ^{becomes } available,

^{an }

### empi-

### rical law may be found which takes into account the changes ^{in } electronic structure which accom-

### pany alloying.

### Even though ^{detailed } interpretation ^{of } ^{the} hyperfine field data is ^{not } yet possible, ^{these } ^{mea-}

### surements can be of value in studying ^{the } magnetic properties ^{of } ^{atoms } in différent environments in

### alloys. ^{As } ^{an } example ^{the } ^{two } iron sites in orde- red Fe3AI ^{have } already ^{been } ^{cited. } Hyperfine

### field measurements using ^{the } ^{Môssbauer } ^{effect} might ^{be } ^{used } ^{to } ^{test } ^{the model } ^{which } ^{has } ^{been} postulated by ^{Marshall } [14] ^{for } antiferromagnetism

### in dilute alloys. According ^{to } this model there is

### a distribution p(He) ^{of } ^{local } magnetic ^{fields } ^{He } ^{at}

### the magnetic ^{atoms } ^{such that } p(O) ^{is } not zero, i.e. there is ^{a } finite probability ^{that } ^{atoms } ^{will be}

### situated in a region ^{of } ^{zero or } ^{small } ^{fields. } ^{These} spins ^{are } ^{free } ^{to } change their orientation and hence

### give ^{rise } ^{to } ^{a } specific ^{heat } ^{at } ^{low } temperatures.

### Since they ^{are } ^{free } ^{to } flip they ^{have } S >

^{= }

### 0 and no hyperfine ^{field. } ^{The } spins ^{in } large ^{local}

### fields are locked to the crystal and would be expec- ted to show a normal hyperfine field. Hence the

### Môssbauer spectrum ^{of such } ^{an } antiferromagnet

### would show

a### spread ^{in } hyperfine fields, ^{and in} particular ^{an } appreciable ^{number } ^{of nuclei } ^{should}

### be in small fields resulting ^{in }

^{an }

### unsplit line in the - centre of the spectrum. The lower the tempe-

### rature the fewer spins contribute to this centre line and so in principle by measuring ^{its } intensity ^{as a}

### function of temperature ^{the } distribution function

### p(He) could be determined. Beck [15] ^{has made}

### the interesting suggestion that anomalies in the linear term in the specific ^{heat of } more concen-

### trated disordered alloys may arise from a similar mechanism involving ^{a } distribution of local fields acting ^{on } ^{the } ^{atoms.}

### 2. Paramagnétie ^{metals } ^{and } alloys.

^{- }

^{In } ^{these}

### materials the main contributio, ^{is } Ho, the magne- tisation ^{M } is small and the small terms additional to Ho give ^{the } Knight shift. We recognise ^{that}

### there are the following contributions to the Knight

### shift which we shall roughly evaluate for the case

### of vanadium. The polarization ^{of the 4s } ^{conduc-}

### tion electrons, acting through (4), gives ^{the well}

### known result [16]

### where _{xs } is the Pauli susceptibility of the conduc- tion electrons and 03C8(O)B 2 ^{is } averaged ^{over } ^{the}

### Fermi surface and, ^{in } principle, ^{includes } the effects of core polarization produced by polarization ^{in}

### the 4s electrons. The 3d electrons

^{are }

### also pola-

### rized by the external field and this produces ^{a core}

### polarisation ^{and hence } ^{a core } ^{field of}

### 737 where

a### is the field produced by ^{one } ^{Bohr } magneton

### in the 3d electrons and is therefore _{very } roughly

### of the order of 100 kg. Finally ^{we } notice that we

### expect ^{a van } ^{Vleck } susceptibility [17] xvv of the order of (2y2J5A) n(10

^{- }

### n) ^{and this } ^{leads } ^{to } ^{a} field, through (2), ^{of}

### where A is

^{an }

### energy parameter of the order of the width of the 3d band and n is the number of 3d electrons per ^{atom. } Because y2 n/A is of the order of _{xd } and r-3 > _{ad } is about 3 X 10 25 ^{cms-3} it follows that HL is of the same order and may very well bé longer ^{than } ^{He. } The numerical results

### quoted ^{in } (10), (11) ^{and } (12) ^{are } only rough ^{but}

### because we can expect Zd ^{to } ^{be } ^{an } ^{ordér } ^{of } magni-

### tude larger than X, ^{we } ^{conclude } ^{that } ^{in } general

### all three contributions are very roughly compa- rable. W é should however specially emphasize

### the difficulties of estimating (11) ^{and } (12) : ^{we } ^{have}

### previously pointed ^{out } ^{the } ^{weakness } ^{of } ^{our } ^{under-} standing ^{of } ^{core } polarization in metals and the estimate of the Van Vleck susceptibility is also very difficult because it depends sensitively ^{on } ^{the}

### detailed band structure of the metal.

### We conclude tbat the proper interpretation ^{of} Knight ^{shifts } in these metals is very hard indeed.

### The same remark applies ^{to } measurements of the nuclear spin relaxation rate, 1 jT 1. There are three contributions to this relaxation rate corresponding

### to the three contributions to the Knight ^{shift } ^{we}

### labelled Il,,, ^{Hc } ^{and } HL; ^{in } addition there is a

### fourth contribution, ^{of } ^{the } ^{saine } orders, ^{which } ^{has}

### its origin ^{in the } dipole interaction with the 3d elec- trons. This dipole interaction oan contribute to

### scàttering ^{and hence } ^{to } lIT 1 ^{but } ^{not } ^{to } ^{the } Knight

### shift in cubic materials. Notice that for S-like conduction electrons alone this dipole ^{relaxation}

### raté is unimportant because r-3 > 4. _{is very} much smaller thafi B’Y 4,(0)12.

’

### REFERENCES

^{’}

### [1] ^{MARSHALL } (W.), ^{Phys. } ^{Rev., } 1958, 110, 1280.

### [2] ^{HANNA } (S. S.), ^{HEBERLE } (J.), LITTLEJOHN (C.), ^{PER-}

Low

### (G. J.), ^{PRESTON } (R. S.) ^{and } ^{VINCENT } (D. H.), Phys. ^{Rev. } Letters, 1960, 4, ^{177. } ^{HANNA } (S. S.),

### HEBERLE (J.), ^{PERLOW } (C. J.), ^{PRESTON } (R. S.) ^{and}

### VINCENT (D. H.), Phys. ^{Rev. } Letters, 1960, 4, ^{513.}

### [3] ^{PERLOW } (G. J.), ^{to be } published.

### [4] ^{ABRAGAM } (A.), ^{HOROWITZ } (J.) ^{and PRYCE } (M. ^{H. } L.),

### Proc. Roy. Soc., 1955, ^{A } 230,169.

### [5] ^{WATSON } (R. E.) and FREEMAN (A. J.), Phys. Rev., 1961, 123, 2027.

### [6] ^{MARSHALL } (W.), ^{Proc. } Phys. Soc., 1961, 78, ^{113.}

### [7] ^{ANDERSON } (P. W.), Phys. Rev.,1941, 124, 41.

### [8] ^{YOSIDA } (K.), private communication.

### [9] ^{GOSSARD } (A. C.), ^{JACCARINO } (V.) ^{and } ^{WERNICK } (J. H.),

### Proc. Int. Conf.

on### Magnetism ^{and } Crystallography, Kyoto, 1961..

### [10] ^{ROBERTS } (L. D.) and THOMSON (J. O.), Bull. Amer.

### Phys. Soc., 1962, 7, ^{351 } and Proc VIIIth Inter- national Conference

on ### Low Temperature Physics, London, 1962, ^{to be } published.

### [11] ^{JOHNSON } (C. E.), ^{RIDOUT } (M. S.) and CRANSHAW

### (T. E.), Proceedings ^{of the } ^{Second } International Conference

on ### the Mossbauer effect, Saclay, 1961, and to be published.

### [12],NATHAN (R.), ^{PIGGOTT } (M. T.) ^{and SHULL } ^{(C. G.),}

### J. Phys. ^{Chem. } Solids, 1958, 6, ^{38.}

### [13] ^{SXULL } (C. G.) and WILKINSON (M. K.), Phys. Rev., 1955, 97, ^{304.}

### COLLINS (M. F.), ^{JONES } (R. V.) ^{and LOWDE } (R. D.),

### Proc. Int. Conf.

on### Magnetism ^{and } Crystallography, Kyoto, ^{1961. } M. F. CoLLINS and J. B. FORSYTHE,

### to be published.

### [14] ^{MARSHALL } (W.), Phys. Rev., 1960, 118, 1519.

### [15] ^{BECK } (P. A.), Private communication.

### [16] e,g. KNIGHT (W. D,), Solid State Physics, ^{Academic} Press, N. Y., 1956, ^{vol. 2.}

### [17] ^{ORGEL } (L. E.), ^{J. } Phys. ^{Chem. } Solids, 1961, 21, 123.

### [18] ^{BOYLE } (A. ^{J. } F.), ^{BUNBURY } (D. ^{St. } P.) and EDWARDS

### (C.), Phys. ^{Rev. } Letters, 1960, 5, ^{553.}

### [19] SHIQLEY (D. A.), Private communication.

### [20] ^{SAMOILOV } (B. N.), SKLYAREVSII (V. V.) and STEPANOV

### (B. P.), ^{Soviet } Physics JETP, 1960, 11, ^{261.}

### SAMOILOV (B. N.), SKLYAREVSII (V. V.) ^{and } GOQOB-

CHENKO